- Nano Express
- Open Access

# Effect of Doping on Hydrogen Evolution Reaction of Vanadium Disulfide Monolayer

- Yuanju Qu
^{1, 2, 3}, - Hui Pan
^{1}Email author, - Chi Tat Kwok
^{2, 1}and - Zisheng Wang
^{3, 1}

**Received: **3 November 2015

**Accepted: **1 December 2015

**Published: **10 December 2015

## Abstract

As cheap and abundant materials, transitional metal dichalcogenide monolayers have attracted increasing interests for their application as catalysts in hydrogen production. In this work, the hydrogen evolution reduction of doped vanadium disulfide monolayers is investigated based on first-principles calculations. We find that the doping elements and concentration affect strongly the catalytic ability of the monolayer. We show that Ti-doping can efficiently reduce the Gibbs free energy of hydrogen adsorption in a wide range of hydrogen coverage. The catalytic ability of the monolayer at high hydrogen coverage can be improved by low Ti-density doping, while that at low hydrogen coverage is enhanced by moderate Ti-density doping. We further show that it is much easier to substitute the Ti atom to the V atom in the vanadium disulfide (VS_{2}) monolayer than other transitional metal atoms considered here due to its lowest and negative formation energy. It is expected that the Ti-doped VS_{2} monolayer may be applicable in water electrolysis with improved efficiency.

## Keywords

- VS
_{2}monolayers - Doping
- Hydrogen production
- Hydrogen evolution reduction
- First-principles calculation

## Background

Two-dimensional (2D) transitional metal dichalcogenide monolayers have received increasing attention because of their amazing physical, chemical, electronic, and magnetic properties [1–8]. The transition-metal dichalcogenides have the formula of MX_{2} (M is a transition metal element from groups IV to VI, and X is a chalcogen element), where one M-atom layer is sandwiched between two X-atom layers [1]. These 2D monolayers have been extensively investigated for possible applications in many areas of science and technology, from nanodevices, photoelectronics, catalysts, to the bioscience [9–17]. Their application as catalysts for hydrogen production in water electrolysis is particularly interesting because of their features, such as low cost, easy large-scale fabrication, and rich abundance on Earth [8, 11, 18–31]. Numerous studies have shown that the catalytic performance of 2D MX_{2} nanostructures is closely related to their conductivity and active sites at edges [18–33]. For example, the metallic edges of MoS_{2}, such as the zigzag edge, are active for hydrogen evolution reaction (HER) in water electrolysis [28–32]. Metallic MX_{2} showed better catalytic activity than its semiconducting counterpart [21, 26]. To enhance the performance, the MoS_{2}/graphene composite had been studied for HER because graphene may improve the conductivity and modify their morphologies [24, 27]. Recently, Pan reported that vanadium disulfide (VS_{2}) monolayer shows the best HER performance in the considered systems and its catalytic activity depends on the hydrogen coverage during HER, which is reduced at high coverage due to the change of conductivity [19]. Kong et al. reported that doping is one of possible methods to improve their activity [28]. In this work, we investigate the effect of doping on the catalytic activity of the VS_{2} monolayer to improve the HER performance on the basis of first-principles calculation. A series of elements, including Ti, Nb, W, Ta, Mo, Pt, Fe, Co, and Ni, are systematically studied. We find that Ti is the best element to easily substitute V in the VS_{2} monolayer and improve the HER ability. We also show that the doping effect on HER strongly depends on the concentration of dopants.

## Methods

The design of catalysts for water electrolysis is based on the first-principles calculation. The hydrogen evolution reduction of the VS_{2} monolayer with the dopant is investigated to improve its catalytic ability. The Vienna Ab initio Simulation Package (VASP) [34] incorporated with the projector augmented wave (PAW) scheme [35, 36], which is based on the density functional theory (DFT) [37] and the Perdew-Burke-Ernzerhof generalized gradient approximation (PBE-GGA) [38], is used in our calculations. Supercells with lattices larger than 10 Å are used to investigate the doping effect and hydrogen-density-dependent HER ability. A 3 × 3 × 1 grid for k-point sampling, based on the Monkhorst and Pack scheme [39], for geometry optimization of supercells, and an energy cutoff of 450 eV are consistently used in our calculations. Densities of states (DOSs) are calculated based on a k-point sampling of 5 × 5 × 1. To avoid image-image interaction between two monolayers in neighboring supercells in the vertical direction, a vacuum region of at least 20 Å is used for separation. Good convergence is obtained with these parameters, and the total energy was converged to 2.0 × 10^{−5} eV/atom. Both of spin-unpolarized and spin-polarized calculations are carried out.

## Results and Discussion

_{2}monolayer with one surface fully covered by hydrogen atoms (

*a*= 3.27 Å) [19] (Fig. 1 and Additional file 1: Figure S1), where the S–H bond length is about 1.37 Å. Two supercells with 3 × 3 × 1 and 4 × 4 × 1 unit cells (331 and 441 supercells, respectively) are used to investigate the effect of the doping concentration. Nine transition metal (TM) elements, including Ti, Nb, W, Ta, Mo, Pt, Fe, Co, and Ni, are considered as dopants in our calculations. To realize the doping, one or two V atoms in the supercells are substituted by TM atoms (Fig. 1c). The doped systems are fully relaxed to study the doping possibility and their HER performance.

_{H}) [19, 40–43] is calculated as the following equation:

_{H}is the hydrogen chemisorption energy defined as:

*n*is the number of H atoms adsorbed on a MX

_{2}monolayer and changed from 1 to 9 (for full hydrogen coverage on the 331 supercell) (Fig. 1a, b) or 1 to 16 (for full hydrogen coverage on the 441 supercell) to investigate the effect of hydrogen coverage on catalytic activity. The hydrogen coverage refers to \( \frac{n}{9} \) (in the 331 supercell) or \( \frac{n}{16} \) (in the 441 supercell). Full coverage refers to each S atom on one side of the VS

_{2}monolayer that is attached with one H atom. Therefore, ΔG

_{H}as a function of the hydrogen coverage can be obtained. E(VS

_{2}+

*n*H), E(VS

_{2}), and E(H

_{2}) in Eq. (2) are the energies of the monolayer with hydrogen atoms (

*n*), pure VS

_{2}monolayer, and hydrogen molecule, respectively. ΔS

_{H}is the difference in entropy. The entropy of adsorption of 1/2 H

_{2}is \( \Delta {\mathrm{S}}_{\mathrm{H}}\cong -1/2{\mathrm{S}}_{{\mathrm{H}}_2}^0 \), where \( {\mathrm{S}}_{{\mathrm{H}}_2}^0 \) is the entropy of H

_{2}in the gas phase at standard conditions. ΔE

_{ZPE}is the difference in zero point energy between the adsorbed and the gas phase, related to the reaction 1/2H

_{2}(g) → H *, where H* denotes a hydrogen atom adsorbed on the surface. ΔE

_{ZPE}− TΔS

_{H}is about 0.24 eV [19, 40–43]. So, Eq. (1) is simplified to ΔG

_{H}= ΔE

_{H}+ 0.24.

_{H}. The relaxed structures show that their geometry are stable and hydrogen atoms keep on the tops of S atoms with the S–H bond of 1.37 Å (Additional file 1: Figure S2). We first study the 331 supercell with one V atom replaced by one TM atom, which is corresponding to a doping concentration of \( \frac{1}{9} \). The calculated Gibbs free energies for hydrogen adsorption on the 331 supercell show that the catalytic activities of doped VS

_{2}monolayers are still dependent on the hydrogen coverage, which decrease with the increment of hydrogen density (Fig. 2). Compared with a pure VS

_{2}monolayer, we see that doping can partially improve its catalytic activity at a certain range of hydrogen density as indicated by the reduced ΔG

_{H}(Fig. 2). For example, the Ni-doped VS

_{2}monolayer shows better HER performance than a pure one in ranges of hydrogen density from \( \frac{3}{9}\kern0.37em \mathrm{t}\mathrm{o}\;\frac{4}{9} \) and from \( \frac{6}{9}\kern0.37em \mathrm{t}\mathrm{o}\;\frac{8}{9} \) (Fig. 2a). Pt-doping and Ti-doping improve the performance in hydrogen density ranging from \( \frac{6}{9}\kern0.37em \mathrm{t}\mathrm{o}\;\frac{8}{9} \) (Fig. 2b) and from \( \frac{1}{9}\kern0.37em \mathrm{t}\mathrm{o}\;\frac{5}{9} \) (Fig. 2c). Interestingly, we see that ΔG

_{H}for W-doped VS

_{2}at the full hydrogen coverage is almost close to zero (0.09 eV) (Fig. 2c). In all of the considered doping elements, we see that Ni- and Ti-doping can improve the HER performance of the VS

_{2}monolayer in a wide hydrogen coverage and W-doping can dramatically enhance its catalytic activity at a high hydrogen coverage. For comparison, we put the calculated ΔG

_{H}of Ni-, Ti-, and W-doped VS

_{2}monolayers as a function of hydrogen density together (Fig. 3a). Clearly, Ti-doping is better than Ni-doping on the HER performance in a range of \( \frac{1}{9}\kern0.37em \mathrm{t}\mathrm{o}\;\frac{5}{9} \), while Ni-doping is better than Ti-doping in a range of \( \frac{6}{9}\kern0.37em \mathrm{t}\mathrm{o}\;\frac{8}{9} \) (Fig. 3a). W-doping is the best at the full hydrogen coverage. The relaxed structure of the W-doped VS

_{2}monolayer with full hydrogen coverage shows that one of the H atoms moves away from the surface around the W-doping site and bonds to other H atoms nearby (inset in Fig. 3a), where the S–H and H–H bond lengths are 1.662 and 0.983 Å, respectively. We also investigate the effect of spin-polarization on the HER performance of the Ti-doped system. We find that spin-polarization may affect slightly the calculated Gibbs free energy at a lower hydrogen coverage but is negligible as the hydrogen coverage increases (Fig. 4). Therefore, spin-polarization is not considered below.

To investigate the effect of the doping concentration on the HER performance, the increment and reduction of the doping density are achieved by replacing more V atoms in the same supercell and enlarging the size of the supercell, respectively. For example, we replace two V atoms using two TM (Ti, Ni, or W) atoms in the 331 supercell, which is equivalent to a doping density of 22.22 % \( \left(\frac{2}{9}\right) \). The calculated Gibbs free energies show that increasing the doping density makes the HER performance worse, indicating that a high doping concentration is not good in application (Additional file 1: Figure S3). Then, we use a 441 VS_{2} supercell with one V substituted by one TM atom (TM = Ti, Ni, and W), which equals to a doping density of about 6.25 % \( \left(\frac{1}{16}\right) \). Clearly, the TM-doping can improve the HER performance of the VS_{2} monolayer under high-H coverage in a range of \( \frac{8}{16}\;\mathrm{t}\mathrm{o}\;\frac{16}{16} \) (Fig. 3b). The catalytic abilities of Ti- and Ni-doped systems are enhanced by 50 % in the hydrogen coverage from \( \frac{8}{16}\;\mathrm{t}\mathrm{o}\;\frac{11}{16} \) (Fig. 3b). However, Ni-doping reduces its performance in hydrogen coverages less than \( \frac{8}{16} \). The catalytic ability of the Ti-doped VS_{2} monolayer at low hydrogen coverages is comparable with or slightly worse than that of the pure VS_{2} monolayer. Similarly, W-doping in the 441 supercell can only improve the HER performance at certain hydrogen densities, such as \( \frac{9}{16}\;\mathrm{and}\;\frac{16}{16} \) (Fig. 3b). The relaxed structure of W-doped VS_{2} with the full hydrogen coverage shows that hydrogen atoms around the doping site move together to form a triangle with a H–H bond length of 1.00 Å and an extended S–H length of 1.90 Å (inset in Fig. 3b). From the calculated Gibbs free energies, we see that Ti is the best candidate as a dopant to improve the HER performance of the VS_{2} monolayer. Comparing with other MX_{2} monolayers, we see that the basal plane of the Ti-doped VS_{2} monolayer has better catalytic performance under the same condition (ΔG_{H} = −0.19 eV at 6.25 % coverage) than that of pure 1T-WS_{2} (ΔG_{H} = 0.28 eV) [21]. It is also worth noting that after doping Ti, Ni, and W atoms individually into the VS_{2} monolayer, the catalytic ability of the basal plane on the doped VS_{2} monolayer has improved dramatically at certain hydrogen coverages, which are equivalent to or even better than that of the active edges sites of MoS_{2}, MoSe_{2}, WS_{2}, and WSe_{2} under the same hydrogen coverages [20]. For example, the catalytic activity of the Ti-doped VS_{2} monolayer (its ΔG_{H} equals −0.05 eV under a hydrogen coverage of \( \frac{2}{9} \) (22.2 %)) is comparable to or better than that at the edges of MoS_{2}, MoSe_{2}, WS_{2}, and WSe_{2} (the optimal ΔG_{H} is from −0.06 to 0.06 eV under a hydrogen coverage of 25 %).

_{2}monolayer under various hydrogen coverages near Fermi levels are mainly contributed to Ti-d and V-d electrons (Figs. 5 and 6). In the 331 supercell, localized defect states near the Fermi level are formed at high hydrogen coverage (Fig. 5c, d), which may lead to reduced carrier mobility and HER performance (Fig. 3a). However, the doping states near the Fermi level in the 441 supercell are connected to the valence band (Fig. 6c, d), resulting in better carrier mobility and improved catalytic activity at high hydrogen coverages (Fig. 3b).

_{2}monolayer, another important issue, which is the doping ability, needs to be stated. The possibility for the dopant to substitute the V atom in the host can be investigated by calculating the formation energy as below:

_{2}+

*n*TM) and E(VS

_{2}) are the total energies of VS

_{2}monolayer supercells with and without dopants.

*μ*

_{TM}and

*μ*

_{V}are the energies of TM and V atoms, respectively.

*n*is the number of dopants in each supercell (

*n*= 1). Our calculations show that the formation energies for Ti-, Mo-, Nb-, and Ta-doping are negative, indicating the reactions are exothermic, while the doping of W, Fe, Co, Ni, and Pt are endothermic because of their positive formation energies (Fig. 7). Particularly, it is easy to substitute the Ti atom to the V atom in the 331 supercell of the VS

_{2}monolayer because of its lowest formation energy (−0.83 eV) (Fig. 7a). W-doping may be achieved under suitable conditions because its endothermic energy is as low as 0.06 eV. Compared with other elements, however, Ni-doping should be difficult because large energy is required (E

_{ f }= 1.88 eV). We further see that their formation energies are reduced if the doping density decreases (Fig. 7b). In this case, the energies of Ti- and W-substitutions are reduced to −1.14 and 0.005 eV, respectively, at a doping density of 6.25 % \( \left(\frac{1}{16}\right) \) (Fig. 7b), indicating that doping at a low concentration is easier than that at a high concentration.

## Conclusions

We present a first-principles study on the effect of doping on the hydrogen evolution reaction of the VS_{2} monolayer. We find that the catalytic activity of the doped VS_{2} monolayer depends strongly on the choice of dopant and the doping concentration. The catalytic ability of the VS_{2} monolayer under high hydrogen coverages can be dramatically enhanced by TM-doping at a low concentration, while that under low hydrogen coverages can be improved by the doping at a moderate density. High-density doping results in reduced HER activity. We further show that Ti-doping should be the best to improve the HER ability of VS_{2} monolayers in our considered doping elements because of the reduced Gibbs free energy at a wide range of hydrogen coverages. By investigating the formation energy of TM substitution of the V atom, we find that the reaction of Ti-substitution of V in the VS_{2} monolayer is exothermic and easier than other TM elements due to its lowest formation energy. It is predicted that the Ti-doped VS_{2} monolayer may show better HER performance and find applications as catalysts in water electrolysis.

## Declarations

### Acknowledgements

Hui Pan thanks the supports of the Science and Technology Development Fund from Macao SAR (FDCT-068/2014/A2, FDCT-132/2014/A3, and FDCT-110/2014/SB) and Multi-Year Research Grants (MYRG2014-00159-FST and MYRG2015-00017-FST) and Start-up Research Grant (SRG-2013-00033-FST) from the Research & Development Office at the University of Macau. The DFT calculations were performed at High Performance Computing Cluster (HPCC) of Information and Communication Technology Office (ICTO) at the University of Macau.

**Open Access**This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.

## Authors’ Affiliations

## References

- Chhowalla M, Shin HS, Eda G, Li LJ, Loh KP, Zhang H (2013) The chemistry of two-dimensional layered transition metal dichalcogenide nanosheets. Nat Chem 5:263–275View ArticleGoogle Scholar
- Gao DQ, Si MS, Li JY, Zhang J, Zhang ZP, Yang ZL, Xue DS (2013) Ferromagnetism in freestanding MoS
_{2}nanosheets. Nanoscale Res Lett 8:129View ArticleGoogle Scholar - Pan H, Zhang YW (2012) Tuning the electronic and magnetic properties of MoS
_{2}nanoribbons by strain engineering. J Phys Chem C 116:11752–11757View ArticleGoogle Scholar - Li XD, Wu SQ, Zhou S, Zhu ZZ (2014) Structural and electronic properties of germanene/MoS
_{2}monolayer and silicone/MoS_{2}monolayer superlattices. Nanoscale Res Lett 9:110View ArticleGoogle Scholar - Mao XZ, Xu Y, Xue QX, Wang WX, Gao DQ (2013) Ferromagnetism in exfoliated tungsten disulfide nanosheets. Nanoscale Res Lett 8:430View ArticleGoogle Scholar
- Pan H (2014) Electronic and magnetic properties of vanadium dichalcogenides monolayers tuned by hydrogenation. J Phys Chem C 118:13248–13253View ArticleGoogle Scholar
- Song XF, Hu JL, Zeng HB (2013) Two-dimensional semiconductors: recent progress and future perspectives. J Mater Chem C 1:2952–2969View ArticleGoogle Scholar
- Wu ZZ, Fang BZ, Wang ZP, Wang CL, Liu ZH, Liu FY, Wang W, Alfantazi A, Wang DZ, Wilkinson DP (2013) MoS
_{2}nanosheets: a designed structure with high active site density for the hydrogen evolution reaction. ACS Catal 3:2101–2107View ArticleGoogle Scholar - Gianluca F, Francesco B, Giuseppe I, Tomas P, Daniel N, Seabaugh AS, Banerjee SK, Colombo L (2014) Electronics based on two-dimensional materials. Nat Phys 9:768–779Google Scholar
- Lemme MC, Li LJ, Palacios T, Schwierz F (2014) Two-dimensional materials for electronic applications. MRS Bul 39:711–718View ArticleGoogle Scholar
- Yan Y, Xia BY, Xu ZC, Wang X (2014) Recent development of molybdenum sulfides as advanced electrocatalysts for hydrogen evolution reaction. ACS Catal 4:1693–1705View ArticleGoogle Scholar
- Namgung SD, Yang S, Park K, Cho AJ, Kim HJ, Kwon JY (2015) Influence of post-annealing on the off current of MoS
_{2}field-effect transistors. Nanoscale Res Lett 10:62View ArticleGoogle Scholar - Kou ZY, Wang X, Yuan RS, Chen HB, Zhi QM, Gao L et al (2014) A promising gene delivery system developed from PEGylated MoS
_{2}nanosheets for gene therapy. Nanoscale Res Lett 9:587View ArticleGoogle Scholar - Ge J, Ou EC, Yu RQ, Chu X (2014) A novel aptameric nanobiosensor based on the self-assembled DNA-MoS
_{2}nanosheet architecture for biomolecule detection. J Chem Mater B 2:625–628View ArticleGoogle Scholar - Pan H (2014) Magnetic and electronic evolutions of hydrogenated VTe
_{2}monolayer under tension. Sci Rep 4:7524View ArticleGoogle Scholar - Klots AR, Newaz AKM, Wang B, Prasai D, Krzyzanowska H, Lin JH, Caudel D et al (2014) Probing excitonic states in suspended two-dimensional semiconductors by photocurrent spectroscopy. Sci Rep 4:6608View ArticleGoogle Scholar
- Gu WX, Yang F, Wu C, Zhang Y, Shi MY, Ma XY (2014) Fabrication and investigation of the optoelectrical properties of MoS
_{2}/CdS heterojunction solar cells. Nanoscale Res Lett 9:662View ArticleGoogle Scholar - Qu YJ, Pan H, Kwok CT, Wang ZS (2015) A first-principles study on the hydrogen evolution reaction of VS
_{2}nanoribbons. Phys Chem Chem Phys 17:24820–24825View ArticleGoogle Scholar - Pan H (2014) Metal dichalcogenides monolayers: novel catalysts for electrochemical hydrogen production. Sci Rep 4:5348Google Scholar
- Tsai C, Chan K, Pedersenb FA, Nørskov JK (2014) Active edge sites in MoSe
_{2}and WSe_{2}catalysts for the hydrogen evolution reaction: a density functional study. Phys Chem Chem Phys 16:13156View ArticleGoogle Scholar - Voiry D, Yamaguchi H, Li JW, Silva R, Alves DCB, Fujita T, Chen MW, Asefa T, Shenoy VB, Eda G, Chhowalla M (2013) Enhanced catalytic activity in strained chemically exfoliated WS
_{2}nanosheets for hydrogen evolution. Nat Mater 13:850–855View ArticleGoogle Scholar - Chena TY, Chang YH, Hsub CL, Weib KH, Chiang CY, Lia LJ (2013) Comparative study on MoS
_{2}and WS_{2}for electrocatalytic water splitting. Int J Hydro Energy 38:12302–12309View ArticleGoogle Scholar - Lukowski MA, Daniel AS, English CR, Meng F, Forticaux A, Hamers RJ, Jin S (2014) Highly active hydrogen evolution catalysis from metallic WS
_{2}nanosheets. Energy Environ Sci 7:2608–2613View ArticleGoogle Scholar - Xia XH, Zheng ZX, Zhang Y, Zhao XJ, Wang CM (2014) Synthesis of MoS
_{2}-carbon composites with different morphologies and their application in hydrogen evolution reaction. Int J Hydrogen Energy 39:9638–9650View ArticleGoogle Scholar - Yang J, Shin HS (2014) Recent advances in layered transition metal dichalcogenides for hydrogen evolution reaction. J Mater Chem A 2:5979–5985View ArticleGoogle Scholar
- Lukowski MA, Daniel AS, Meng F, Forticaux A, Li LS, Jin S (2013) Enhanced hydrogen evolution catalysis from chemically exfoliated metallic MoS
_{2}nanosheets. J Am Chem Soc 135:10274–10277View ArticleGoogle Scholar - Min SX, Lu GX (2012) Sites for high efficient photocatalytic hydrogen evolution on a limited-layered MoS
_{2}cocatalyst confined on graphene sheets—the role of graphene. J Phys Chem C 116:25415–25424View ArticleGoogle Scholar - Kong DS, Cha JJ, Wang HT, Lee HR, Cui Y (2013) First-row transition metal dichalcogenide catalysts for hydrogen evolution reaction. Energy Environ Sci 6:3553–3558View ArticleGoogle Scholar
- Kibsgaard J, Chen Z, Reinecke BN, Jaramillo TF (2012) Engineering the surface structure of MoS
_{2}to preferentially expose active edge sites for electrocatalysis. Nat Mater 11:963–969View ArticleGoogle Scholar - Jaramillo TF, Jørgensen KP, Bonde J, Nielsen JH, Horch S, Chorkendorffl I (2007) Identification of active edge sites for electrochemical H
_{2}evolution from MoS_{2}nanocatalysts. Science 317:100–102View ArticleGoogle Scholar - Karunadasa HI, Montalvo E, Sun YJ, Majda M, Long JR, Chang CJ (2012) Molecular MoS
_{2}edge site mimic for catalytic hydrogen generation. Science 335:698–702View ArticleGoogle Scholar - Pan H, Zhang YW (2012) Edge-dependent structural, electronic and magnetic properties of MoS
_{2}nanoribbons. J Mater Chem 22:7280–7290View ArticleGoogle Scholar - Chen DY, Chen WX, Ma L, Ji G, Chang K, Lee JY (2014) Graphene-like layered metal dichalcogenide/graphene composites: synthesis and applications in energy storage and conversion. Mater Today 17:184–193View ArticleGoogle Scholar
- Kresse G, Furthmuller J (1996) Efficient iterative schemes for ab initio total-energy calculations using a plane-wave basis set. Phys Rev B 54:11169–11186View ArticleGoogle Scholar
- Perdew JP, Burke K, Ernzerhof M (1996) Generalized gradient approximation made simple. Phys Rev Lett 77:3865–3868View ArticleGoogle Scholar
- Kresse G, Joubert D (1999) From ultrasoft pseudopotentials to the projector augmented-wave method. Phys Rev B 59:1758–1775View ArticleGoogle Scholar
- Hohenberg P, Kohn W (1964) Inhomogeneous electron gas. Phys Rev 136:B864–B871View ArticleGoogle Scholar
- Blöchl PE (1994) Projector augmented-wave method. Phys Rev B 50:17953–17979View ArticleGoogle Scholar
- Monkhorst HJ, Pack J (1976) Special points for Brillouin-zone integrations. Phys Rev B 13:5188–5192View ArticleGoogle Scholar
- Gressley J, Jarmaillo TF, Bonde J, Chorkendorff I, Nørskov JK (2006) Computational high-throughput screening of electrocatalytic materials for hydrogen evolution. Nat Mater 5:909–913View ArticleGoogle Scholar
- Pan H, Feng YP, Lin JY (2010) Enhancement of hydrogen evolution on tungsten doped platinum. J Comput Theor Nanosci 7:547–551View ArticleGoogle Scholar
- Nørskova JK, Bligaarda T, Logadottira A, Kitchinb JR, Chenb JG, Pandelovc S, Stimmingc U (2005) Trends in the exchange current for hydrogen evolution. J Electrochem Soc 152:J23–J26View ArticleGoogle Scholar
- Fang YH, Wei GF, Liu ZP (2013) Catalytic role of minority species and minority sites for electrochemical hydrogen evolution on metals: surface charging, coverage, and Tafel kinetics. J Phys Chem C 117:7669–7680View ArticleGoogle Scholar